Vortex ratchet induced by controlled edge roughness

**Vortex** **ratchet** **induced** **by** **controlled** **edge** **roughness**

D Cerbu 1,6 , V N Gladilin 1,2 , J Cuppens 1,5 , J Fritzsche 3 ,

J Tempere 2 , J T Devreese 2 , V V Moshchalkov 1 , A V Silhanek 4

and J Van de Vondel 1

1 INPAC—Institute for Nanoscale Physics and Chemistry, KU Leuven,

Celestijnenlaan 200D, B-3001 Leuven, Belgium

2 TQC—Theory of Quantum and Complex Systems, Universiteit Antwerpen,

Universiteitsplein 1, B-2610 Antwerpen, Belgium

3 Department of Applied Physics, Chalmers University of Technology,

SE-412 96 Göteborg, Sweden

4 Département de Physique, Université de Liège, Allée du 6 août 17, Bat. B5a,

B-4000 Sart Tilman, Belgium

E-mail: dorin.cerbu@fys.kuleuven.be

New Journal of Physics 15 (2013) 063022 (13pp)

Received 8 March 2013

Published 17 June 2013

Online at http://www.njp.org/

doi:10.1088/1367-2630/15/6/063022

Abstract. We demonstrate theoretically and experimentally the generation

of rectified mean vortex displacement resulting from a **controlled** difference

between the surface barriers at the opposite borders of a superconducting strip.

Our investigation focuses on Al superconducting strips where, in one of the two

sample borders, a saw tooth-like array of micro-indentations has been imprinted.

The origin of the vortex **ratchet** effect is based on the fact that (i) the onset

of vortex motion is mainly governed **by** the entrance/nucleation of vortices

and (ii) the current lines bunching produced **by** the indentations facilitates the

entrance/nucleation of vortices. Only for one current direction the indentations

are positioned at the side of vortex entry and the onset of the resistive regime is

lowered compared to the opposite current direction. This investigation points to

the relevance of ubiquitous border effects typically neglected when interpreting

vortex **ratchet** measurements on samples with arrays of local asymmetric pinning

sites.

5 Present address: Department of Condensed Matter Physics, Weizmann Institute of Science, Rehovot 76100, Israel.

6 Author to whom any correspondence should be addressed.

Content from this work may be used under the terms of the Creative Commons Attribution 3.0 licence.

Any further distribution of this work must maintain attribution to the author(s) and the title of the work, journal

citation and DOI.

New Journal of Physics 15 (2013) 063022

1367-2630/13/063022+13$33.00 © IOP Publishing Ltd and Deutsche Physikalische Gesellschaft

2

Contents

1. Introduction 2

2. Sample details 3

3. Experimental results 4

4. Theoretical model 6

5. Calculated results 8

6. Discussion 10

7. Conclusions 11

Acknowledgments 12

References 12

1. Introduction

Mobile physical entities such as particles, bacteria or water droplets, subjected to a zero mean

periodic excitation, can acquire a finite mean momentum if the energy potential landscape is

asymmetric [1–4]. A particularly attractive system for testing these non-equilibrium phenomena

can be made on the basis of type-II superconductors where the quantum bundles of magnetic

flux can be regarded as repulsively interacting particles in an energy potential landscape fully

determined **by** the inhomogeneities of the superconducting condensate [5, 6]. The possibility of

changing the number of particles **by** simply changing the magnetic field intensity or of tuning

the size of the particles **by** properly adjusting the temperature makes this superconducting

system an ideal toy model. In general, for isolated particles, rectification is obtained when

the typical distance traveled **by** the particles during the period of the excitation is larger than

the length scale at which the symmetry of the potential is broken. However, the response

of the system becomes more complex at high densities, when the separation between the

particles is smaller than the length scale of the potential and their mutual interaction becomes

important. For instance, multiple reversals of the easy-axis rectification direction can be

observed as the number of particles is increased or when the characteristic length scale of the

potential asymmetry changes [7–9].

The vast majority of the theoretical approaches for describing the physical mechanisms of

these **ratchet** systems assume an infinite medium with no borders or with periodic boundary

conditions. Neglecting sample borders in superconducting systems seems to be unjustified from

an experimental point of view [10, 11] unless special care is taken to move the particles in

circles such as in the Corbino disc configuration [12]. Indeed, it has been recognized in the past

that unwanted differences between the two sample borders can lead to spurious rectification

signals [13–17]. However, it still remains unclear whether there is also an influence from the

asymmetric entering–exit process.

More than 50 years ago the work of Bean and Livingstone (BL) addressed the influence of

the sample **edge** on the magnetic properties of a type-II superconductor [18]. In their seminal

paper, they describe the presence of a surface barrier at a vacuum/superconducting interface

arising from the competition between the repulsion of a vortex from the surface due to Meissner

currents, and the attractive image force arising from the boundary condition of zero current

normal to the sample **edge**.

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

3

This surface barrier, inherently present in finite superconducting samples, is not symmetric,

i.e. the energy needed to introduce a vortex into the sample is different from that needed to

remove the vortex from the sample. This difference between vortex nucleation and vortex exit

leads to metastabilities that manifest themselves as hysteretic magnetization curves [19, 20].

Although in electrical transport experiments the BL barrier can be an important factor that

determines the critical current (particularly in the weak pinning regime), the fact that vortex

trajectories involve entering, traveling across the sample and exiting the sample implies that the

most resistive mechanism (i.e. vortex entering) dominates. This asymmetry of the BL barrier

could not yet be detected with ac transport measurements since, once again, both the entering

and exiting processes take place at the same time for the vortex lattice independent of the current

direction.

We will show that even though the asymmetry of the BL barrier does not constitute a

sufficient condition to induce vortex rectification **by** electrical transport measurements, it is a

necessary ingredient to achieve rectification. It is possible to create a vortex rectifier **by** lowering

the barrier for vortex entry only on one side of the superconducting bridge while leaving the

other side unchanged. Depending on the sign of the applied current, vortex entry can occur

either at one or the other side of the bridge. As a result, only for one particular current direction

the barrier for vortex entry is drastically reduced, which is manifested in a clear difference

between the measured dissipation for both current directions.

In this paper, we study the impact of a micro fabricated **roughness** at the border of a

superconducting thin film on the rectification of vortices. We investigate the difference in dc

voltage (V dc ) response under an ac current drive, between a superconducting Al bridge with two

equally straight **edge**s and a bridge with an array of indentations only on one side of the bridge.

The size of these saw tooth indentations has been chosen to be comparable with the size of

the superconducting vortices. The experimental findings are in agreement with time-dependent

Ginzburg–Landau (TDGL) simulations.

2. Sample details

We investigate superconducting Al thin films in strip geometry of 50 µm width, 200 µm length

and 50 nm thickness. The fabrication was done **by** patterning a resist mask, on top of a SiO 2

substrate, with the help of electron beam lithography and then **by** deposition of an Al thin

film **by** molecular beam epitaxy on top of the patterned resist mask and subsequent lift-off.

Only at one side of the bridge a series of equally spaced triangular-shaped indentations were

made. The dimensions of the fabricated samples are presented in figure 1. In order to check

reproducibility and robustness of this type of vortex rectifier, we fabricated several samples

with varying density of indentations. We focus here on the two extreme cases: the reference

bridge with no indentations and the bridge with one indented side with maximum density of

indents allowed **by** their size, having zero pitch between the indents.

According to the Drude model [21] the product ρl el is a constant that depends on

the material, where ρ and l el are resistivity and electron mean free path, respectively.

In [22] it has been shown that for thin aluminum films we have ρ 4 K l el = 4 × 10 −16 m 2 .

In our case the measured resistivity at 4 K is ρ 4 K = 1.425 × 10 −8 m, which gives l el =

28 nm. The dirty limit expressions [23] ξ(T ) = 0.855 √ ξ(0)l el /(1 − T/T c0 ) and λ(T ) =

0.64λ L (0) √ ξ(0)/l el (1 − T/T c0 ), where λ L (0) is the London penetration depth, result in a

coherence length ξ(0) = 181 nm and a penetration depth λ(0) = 77 nm for the samples under

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

4

Figure 1. Superconducting aluminum thin film in bridge geometry. The side

contacts are used for voltage probing and the current is injected through

the contact pads at each end of the bridge. The geometrical parameters are

a = 2.5 µm, b = 50 µm, c = 200 µm and Al film thickness t = 50 nm. H, J

and F L are the applied magnetic field, the driving current density and the

Lorentz force acting upon Abrikosov vortices, respectively. The directions of

the magnetic field and driving current, as illustrated here, give the definitions for

the positive applied values. At the right side of the figure, we have an atomic

force microscopy image of the flat side of the Al bridge. The nominally flat

border has imperfections such as protrusions sticking out **by** 0.25 µm. The red

dashed lines illustrate for comparison the shape and size of the indents at the

opposite side of the bridge.

investigation. The effective penetration depth (0) = λ 2 (0)/t for the t = 50 nm thin film is

(0) = 119 nm. The critical temperature, determining the onset of superconductivity, is T c0 =

1.285 K.

3. Experimental results

The electrical measurements were carried out using a four-probe Kelvin configuration, with

ac currents fed **by** a Keithley 6221 source whereas a Keithley 1228a digital nanovoltmeter

was used for voltage probing. The E dc ( j ac ) characteristics for the studied samples are shown

in figure 2. Here the applied magnetic field is 0.55 mT and the frequency of the ac current

is f = 33.711 kHz. Taking into consideration that typically the vortex velocities are at least

hundreds of meters per second [24], for micrometer-wide bridges the low applied driving

frequency ensures that during half of the ac cycle the vortices travel across the entire bridge. The

measurement was taken at temperature T = 1.12 K (0.87 T/T c0 ). The inset of figure 2 shows a

zoom-in at lower current densities where the generated electrical field E dc corresponds to a

vortex **ratchet** and the easy direction of vortex **ratchet** motion is from left to right (see figure 1)

in the indented bridge. The reference sample shows no vortex **ratchet** effect. In figure 2, we can

clearly distinguish an E dc peak at a current density roughly 30 kA cm −2 for the indented sample

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

5

Figure 2. Comparison of the electric field–current E dc ( j ac ) characteristics for

the reference and the indented samples. The inset shows a zoom of E dc ( j ac ) for

low current density values at the onset of the resistive regime. Measurements

were done in a magnetic field perpendicular to the film surface H = 0.55 mT

and for a driving frequency f = 33.711 kHz. The cryostat temperature during

measurements was kept at T = 1.12 K.

Figure 3. Contour plot, for the reference and indented samples, of the net dc

electric field E dc ( j ac , H) as a function of the magnetic field and amplitude of

the sinusoidal ac current density at a frequency 33 kHz and T/T c0 = 0.87. The

dashed lines at H = 0.55 mT indicate the conditions under which the data of

figure 2 were obtained.

(open squares) and a much smaller peak at roughly 32 kA cm −2 for the reference sample (filled

circles). The steep increase of E dc has been attributed to the onset of phase slip lines (PSLs)

once the vortex velocity reaches a critical value [25].

In figure 3 we have for both samples the obtained electric field versus current density

E dc ( j ac ) measurements taken at T = 1.12 K for different magnetic fields ranging from −0.8

to 0.8 mT. These contour plots clearly demonstrate that the presence of indents induces the

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

6

rectification of vortex motion over a wide range of magnetic fields. In contrast to that,

the reference sample exhibits a very weak rectification signal probably originating from

unavoidable imperfections of the nominally flat sample borders, in agreement with previous

reports [13, 14, 26] or from the fact that placing both voltage contacts at one side of the bridge

leads also to breaking the inversion symmetry [27, 28].

The antisymmetric dependence on the magnetic field is explained **by** the inversion of the

Lorentz force (and therefore also the vortex motion direction) when changing the polarity of

the magnetic field-**induced** vortices. The rectification sign for all indented samples is identical,

which indicates that the easy direction of vortex motion in these samples is the same. This shows

that the indentations break the symmetry of vortex motion in a robust and systematic way.

4. Theoretical model

We describe vortex dynamics using the generalized TDGL equation for dirty superconductors

[29]:

(

1 ∂

√

1 + γ

2

|ψ| 2 ∂t + iϕ + 1 )

2 γ 2 ∂|ψ|2 ψ

∂t

= (∇ − iA) 2 ψ + 2

(1 − T )

ψ(1 − |ψ| 2 ). (1)

T c

Here ψ is the order parameter, and ϕ and A are the scalar and vector potentials, respectively.

The relevant quantities are made dimensionless **by** expressing lengths in units of √ 2ξ(0), time in

units of π ¯h/(4k B T c ) ≈ 11.6τ GL (0), magnetic field in units of 0 /(4πξ 2 (0)) = H c2 (0)/2, current

density in units of 0 /[2 √ 2πµ 0 λ 2 (0)ξ(0)] = 3 √ 3/(2 √ 2) j c (0) and scalar potential in units of

2k B T c /(πe). Here, 0 = π ¯h/e is the magnetic flux quantum, µ 0 is the vacuum permeability, τ GL

is the Ginzburg–Landau time, H c2 is the second critical field and j c is the critical (depairing)

current density of a thin wire or film [23].

The parameter γ = 8τ E k B T c

√ u(1 − T/Tc )/(π ¯h) is proportional to τ E , the inelastic

collision time for electron–phonon scattering. u is a numerical factor, which approximately

equals 5.79 [29]. At γ ≫ 1 the healing time of the superconducting condensate is ∼γ |ψ|τ GL

(see e.g. [30]). Equation (1) is strictly valid for [29] γ 2 < u/(1 − T/T c ), i.e. for γ 10 at

(1 − T/T c ) 0.1. At the same time, the γ value experimentally obtained for Al is as large

as ∼1000 for those temperatures [31]. Nevertheless, it appears that the approach, based on the

use of equation (1) with γ ∼ 10, is able to capture the main physical mechanisms, related to the

vortex dynamics in thin Al samples [32] as well as to the **ratchet** effect in Al bridges with arrays

of asymmetric pinning sites [25]. In the present calculations, we take γ = 10.

The distribution of the scalar potential ϕ that enters in equation (1) is determined from the

condition

∇ · j = 0 (2)

which reflects the continuity of currents in the superconductor. The total current density j is

given **by** the sum of the normal and superconducting components:

j = j n + j s , (3)

j n = − σ 2

(

∇ϕ + ∂A )

, (4)

∂t

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

7

Figure 4. (a) Calculated distribution of the square modulus of the order

parameter in the absence of an applied current. Panels (b) and (c) show the

distributions of the streaming parameter S for t 2 − t 1 = 40 000 at positive ( j dc =

43 kA cm −2 ) and negative ( j dc = −43 kA cm −2 ) applied dc current, respectively.

j s =

(

1 − T T c

) [Im

(ψ ∗ ∇ψ) − A|ψ| 2] , (5)

where σ is the normal-state conductivity, which is taken as σ = 1/12 in our units [33]. The

vector potential A, for which we choose the gauge ∇ · A = 0, can be represented as

A = A e + A s . (6)

Here A e denotes the vector potential corresponding to the externally applied magnetic field H,

while A s describes the vector potential **induced** **by** the currents j that flow in the superconductor:

A s (r) = 1

2πκ 2 ∫

d 3 r ′ j(r ′ )

|r − r ′ | , (7)

where κ = λ/ξ is the Ginzburg–Landau parameter. Integration in equation (7) is performed over

the volume of the superconductor.

In our model, we consider a thin superconducting strip (see figure 4(a)) with

thickness 50 nm, lateral sizes L x × L y = 15 µm × 30 µm (somewhat smaller than those for

the experimental samples) and indentations similar to those in the experimental samples.

An external homogeneous constant magnetic field H is perpendicular to the strip, while the

external transport current is applied in the y-direction. The TDGL simulations are performed for

ξ(0) = 181 nm, λ(0) = 77 nm, T = 1.12 K, T c = 1.285 K and H = 0.55 mT. Since the thickness

of the superconductor is significantly smaller than the coherence length ξ(T ), variations of the

order-parameter magnitude across the layer as well as currents in this direction are negligible.

For such a thin superconductor film, equations (1) and (2) can be rewritten in the xy-plane

only, **by** replacing ∇ with ∇ 2D ≡ e x ∂/∂x + e y ∂/∂y and A with 〈A 2D 〉, where e x and e y are unit

vectors in the x- and y-directions, respectively, while 〈A 2D 〉 denotes the in-plane vector potential

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

8

averaged along the thickness of the superconductor. The superconductor–insulator boundary

conditions

( )

∂

∂x − iA x ψ

∣ = 0, j nx | x=0,L x

= 0 (8)

x=0,L x

which ensure zero values for both the superconducting and normal components of the current

across the boundary, are assumed in the x-direction. In the y-direction, we take the normal

metal–superconductor boundary conditions

ψ| y=0,L y

= 0, j ny

∣

∣y=0,L

y

= j e (9)

with a uniform density of the externally applied current j e at the boundaries.

When solving numerically the two-dimensional (2D) version of the TDGL equation (1),

the gauge invariance of the discretized equations is preserved **by** introducing link variables

following the method of [34, 35]. The 2D grid, used in our calculations, has 123 × 243

equally spaced nodes. As described in more detail in [36], the step h t of the time variable t

is automatically adapted in the course of calculation. This adaptation is aimed at minimizing

the number of steps in t and—at the same time—to keep the solving procedure accurate. In the

present simulations the step h t is typically ∼10 −5 to ∼10 −3 depending on a specific distribution

of the order parameter. For momentary distributions of the order parameter and the (timedependent)

in-plane vector potential 〈A 2D 〉, an iteration procedure is used to determine from

equation (2) the corresponding distribution of the scalar potential ϕ with a relative accuracy

not worse than 10 −4 . The (time-dependent) vector potential 〈A 2D 〉 and the corresponding link

variables are calculated using equation (7).

5. Calculated results

In figure 5(a), the calculated time-averaged electric field E dc = 〈ϕ A − ϕ B 〉/ (y A − y B ) between

points A and B (see figure 5(b)) is shown as a function of the increasing density of the applied

dc | j dc | current for positive (filled circles) and negative (open triangles) current directions. As

seen from the inset of figure 5(a), for positive applied currents (full circles), which cause a

Lorentz force acting on vortices in the positive x-direction, the onset of the resistive regime

occurs at a significantly smaller value of | j dc | than in the case of negative applied currents

(empty triangles), which tend to move vortices in the negative x-direction. This result is

natural, because the indentations, which are present at the left (x = 0) boundary of the strip,

greatly facilitate nucleation of vortices and their entry into the superconductor. Even at current

densities quite above the onset of the resistive regime in the case of flat boundaries, vortex entry

on the micropatterned boundary takes place exclusively through the vertices of indentations.

This is illustrated in figure 4(b), where we plot the distribution of the streaming parameter

S =

[

(t 2 − t 1 ) −1 ∫ t 2

t 1

(∂|ψ| 2 /∂t) 2 dt] 1/2,

introduced in [37] to visualize the vortex trajectories. In

the case of negative applied dc currents, where vortices enter the strip through the flat right

(x = 15 µm) boundary, the entry points for vortices are not well defined. As a result, the

corresponding pattern of S (figure 4(c)) appears somewhat smeared out as compared to that

shown in figure 4(b).

For comparison, in figure 5(a) we also plot the results calculated for a symmetric strip with

flat boundaries at both sides (crosses). As follows from the inset of figure 5(a), in this case

the magnitude of the critical current, which corresponds to the onset of the resistive regime,

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

9

c

e

(a)

b

d

Figure 5. (a) Absolute value of the calculated average electric field E dc between

points A and B (see panel (b)) as a function of the increasing density | j dc | of

the applied dc current for positive (filled circles) and negative (open triangles)

current directions. For comparison, the results for a symmetric bridge with

flat boundaries are shown with crosses. Snapshots of the order parameter

distributions, which correspond to points labeled as ‘b’ ( j dc = 59 kA cm −2 ), ‘c’

( j dc = 94 kA cm −2 ), ‘d’ ( j dc = −87 kA cm −2 ) and ‘e’ ( j dc = −122 kA cm −2 ), are

plotted in panels (b)–(e), respectively. The inset of panel (a) shows the behavior

of E dc ( j dc ) at relatively low current densities.

is practically the same as that for negative currents in the strip with indentations shown in

figure 4. This clearly demonstrates that the onset of the resistive regime is mainly determined

**by** a possibility for vortices to enter the superconductor and hence **by** the properties of the ‘inlet’

boundary of the strip, rather than **by** the properties of the ‘outlet’ boundary. However, as seen

from a comparison between the results plotted in figure 5(a) with crosses and open triangles, the

effect due to patterning of the ‘outlet’ boundary on the behavior of E dc ( j dc ) above the critical

current is not negligible. In particular, such a patterning facilitates the formation of PSLs (see

figures 5(b)–(e)), which results in sudden jumps of E dc versus | j dc | (see figure 5(a)). In the case

of a patterned ‘inlet’ boundary, the PSLs appear at even smaller current densities | j dc |.

The difference between the curves E dc ( j dc ) for positive and negative current directions

(filled circles and open triangles, respectively, in figure 5(a)) implies the appearance of a positive

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

10

Figure 6. Calculated rectified electric field E dc between points A and B (see

figure 5(b)) as a function of the density amplitude j ac of the applied lowfrequency

ac current. The inset shows the behavior of E dc ( j ac ) at relatively low

current densities.

rectified electric field E dc when applying an ac current to the strip. In the limit of low ac

frequencies, this rectified electric field (see figure 6) is found using the results for an increasing

dc current (figure 5(a)) as well as the curves E dc ( j dc ) calculated for decreasing current densities

j dc starting from the values that correspond to different numbers of PSLs (not shown here). A

relatively large difference between the current densities, corresponding to the formation of a

given number of PSLs at positive and negative current directions (see figure 5(a)), results in a

broad peak of E dc ( j ac ) in figure 6. The smaller features on the curve E dc ( j ac ) are related to the

change of the number of PSLs formed during the positive/negative half-period of the applied

ac current.

6. Discussion

Upon comparing the calculated results with the measured data, we find good qualitative

agreement between theory and experiment. In both cases the indented sample manifests a

sizable and robust **ratchet** signal. When comparing figure 6 with figure 2, one can notice that the

steep increase of the calculated E dc ( j ac ), caused **by** the onset of the PSL regime, occurs at an

appreciably higher amplitude of the ac current density j ac than that experimentally observed for

the indented strip. This discrepancy can be attributed to the difference between the used γ = 10

and much larger experimental γ -values for Al (indeed, an increase of γ leads to formation of

PSLs at lower currents—see e.g. [30]). However, the aforementioned difference in γ -values

cannot explain the fact that both the height and the width of the peak in the calculated E dc ( j ac )

are much larger than those observed in the experiment. Indeed, at low ac frequencies an increase

of γ tends to increase the magnitude of the rectified field in the PSL regime [25]. It must be

mentioned that at high vortex velocities heating effects must not be neglected. Heating could

contribute to lowering the currents corresponding to the formation of PSLs for both polarities

of the current, therefore lowering the height and width of the measured **ratchet** signal.

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

11

The difference between the calculated and measured shapes of the E dc ( j ac ) peak may also

be related to the presence of imperfections on the nominally flat **edge**s of the experimental

samples (see figure 1). Indeed, **edge** defects are known to significantly facilitate the vortex

entrance through a rough **edge** [14, 38]. Due to this effect, the difference between the current

densities that correspond to the formation of PSLs for positive and negative currents can be

significantly smaller as compared to our model, where the right **edge** of the superconducting

strip is perfectly flat. Correspondingly, the height and width of the measured E dc ( j ac ) peak

should be reduced as compared to the calculations for an idealized sample. This explanation is

supported **by** the observation of a relatively well pronounced peak of E dc ( j ac ) on the reference

sample with nominally flat boundaries at ac current amplitudes that slightly exceed those for

the indented sample (see figure 2). Remarkably, for both the reference and indented samples

the measured values of the rectified field E dc still remain comparable to or even larger than the

maximum rectified electric fields (few mV cm −1 ) experimentally obtained for **ratchet** systems

with intentionally introduced arrays of asymmetric antidots [9, 39]. This clearly indicates that

the properties of the sample **edge**s may play an important role, also when measuring the rectified

voltage on samples with **ratchet** arrays.

Our TDGL simulations also show that the maximum critical dc current density j 1 ,

corresponding to the onset of vortex propagation across the superconducting bridge shown

in figure 4(a), is achieved at a non-zero magnetic field. This confirms earlier predictions

[13, 14] for the field dependence of the critical current in a superconducting strip with different

vortex-entry conditions at the opposite boundaries. In [13, 14] such different vortex-entry

conditions, attributed to different **roughness**es of the sample boundaries, were introduced ad

hoc **by** postulating an arbitrarily chosen difference between the two critical current densities

for vortex entry at the two opposite sides of the strip. As distinct from the aforementioned

model, in the present model a difference between the surface barriers for vortex entry shows

up as a direct natural consequence of the engineered sample asymmetry. Due to this wellpronounced

asymmetry, in a considerably wide range of magnetic fields around zero the critical

density j 1 of a positive dc current appears to be a monotonously decreasing function of H:

we find j 1 = 282, 231 and 182 kA cm −2 for H = −0.025, 0 and 0.025 mT, respectively. A

relatively large magnitude of the derivative ∂ j 1 /∂ H| H=0 ≈ −2000 kA (cm −2 mT) implies that

an efficient rectification of vortex motion is possible also in the regime where, instead of a dc

magnetic field and an ac current, a weak ac magnetic field and a dc current (e.g. with density

j dc ≈ 230 kA cm −2 ) are applied to the structure under consideration.

7. Conclusions

Summarizing, we report a qualitative and quantitative analysis of rectified electric fields in

indented Al bridges. The origin of the **ratchet** is based on the fact that the onset of vortex motion

is mainly governed **by** the entrance/nucleation of vortices and the current crowding effect

produced **by** the indentations that facilitate this vortex nucleation process. Upon comparing

the calculated results with the measured data we find good agreement between theory and

experiment. In both cases the indented sample exhibits a sizable and robust **ratchet** signal. We

show that the defects at geometrical borders of a superconducting bridge can play a crucial role

in the overall **ratchet** signal. These effects have been systematically ignored when interpreting

the results of **ratchet** effect measurements performed in samples with arrays of asymmetric

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

12

pinning centers. Our findings point to the need of revising previous investigations, particularly

when making quantitative estimations.

Acknowledgments

This work was supported **by** Methusalem funding **by** the Flemish government, the

Flemish Science Foundation (FWO-Vl), in particular FWO projects G.0356.05, G.0115.06,

G.0370.09N and G.0115.12N, the Scientific Research Community project WO.033.09N,

the Belgian Science Policy and the COST MP1201 NanoSC Action. The work

of AVS was partially supported **by** ‘Mandat d’Impulsion Scientifique’ of the FRS-

FNRS and **by** the ‘Crédit de démarrage’ U.Lg. JVdV acknowl**edge**s support from

FWO-Vl.

References

[1] Reimann P 2002 Phys. Rep. 361 57

[2] Hanggi P and Marchesoni F 2009 Rev. Mod. Phys. 81 387

[3] Hanggi P, Marchesoni F and Nori F 2005 Ann. Phys. 14 51–70

[4] Linke H 2002 Appl. Phys. A 75 167

[5] Villegas J E, Savelev S, Nori F, Gonzalez E M, Anguita J V, Garcia R and Vicent J L 2003 Science 302 1188

[6] Van de Vondel J, De Souza Silva C C, Zhu B Y, Morelle M and Moshchalkov V V 2005 Phys. Rev. Lett.

94 057003

[7] de Souza Silva C C, Van de Vondel J, Morelle M and Moshchalkov V V 2006 Nature 440 651

[8] Gillijns W, Silhanek A V, Moshchalkov V V and Reichhardt C 2007 Phys. Rev. Lett. 99 247002

[9] Qiming L, Olson Reichhardt C J and Reichhardt C 2007 Phys. Rev. B 75 054502

[10] Girard J-P, Paumier E and Hairie A 1980 Phys. Rev. B 21 2734

[11] Marchenko V A and Sal’nikov G I 1987 Surface: Physics, Chemistry, Mechanics 3 112 (in Russian)

[12] Lin N S, Heitmann T W, Yu K, Plourde B L T and Misko V R 2011 Phys. Rev. B 84 144511

[13] Plourde B L T, Van Harlingen D J, Vodolazov D Yu, Besseling R, Hesselberth M B S and Kes P H 2001

Phys. Rev. B 64 014503

[14] Vodolazov D Y and Peeters F M 2005 Phys. Rev. B 72 172508

[15] Pryadun V V, Sierra J, Aliev F G, Golubovic D S and Moshchalkov V V 2006 Appl. Phys. Lett. 88 062517

[16] De Souza Silva C C, Silhanek A V, Van de Vondel J, Gillijns W, Metlushko V, Ilic B and Moshchalkov V V

2007 Phys. Rev. Lett. 98 117005

[17] Aliev F G, Levanyuk A P, Villar R, Sierra J F, Pryadun V V, Awad A and Moshchalkov V V 2009

New J. Phys. 11 063033

[18] Bean C P and Livingston J D 1964 Phys. Rev. Lett. 12 14–6

[19] Geim A K, Grigorieva I V, Dubonos S V, Lok J G S, Maan J C, Filippov A E and Peeters F M 1997 Nature

390 259–62

[20] Singha Deo P, Schweigert V A and Peeters F M 1999 Phys. Rev. B 59 6039–42

[21] Drude P 1900 Ann. Phys. 1 566–613

[22] Romijn J, Klapwijk T M, Renne M J and Mooij J E 1982 Phys. Rev. B 26 3648–55

[23] Tinkham M 1996 Introduction to Superconductivity 2nd edn (New York: McGraw-Hill)

[24] Leo A, Grimaldi G, Nigro A, Pace S, Verellen N, Silhanek A V, Gillijns W, Moshchalkov V V, Metlushko V

and Ilic B 2010 Physica C 470 904–6

[25] Van de Vondel J, Gladilin V N, Silhanek A V, Gillijns W, Tempere J, Devreese J T and Moshchalkov V V

2011 Phys. Rev. Lett. 106 137003

[26] Sabatino P, Carapella G and Gombos M 2012 J. Appl. Phys. 112 083909

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)

13

[27] Clem J R, Mawatari Y, Berdiyorov G R and Peeters F M 2012 Phys. Rev. B 85 144511

[28] Adami O-A et al 2013 Appl. Phys. Lett. 102 052603

[29] Kramer L and Watts-Tobin R J 1978 Phys. Rev. Lett. 40 1041

[30] Vodolazov D Y and Peeters F M 2007 Phys. Rev. B 76 014521

[31] Lawrence W E and Meador A B 1978 Phys. Rev. B 18 1154

[32] Vodolazov D Y, Peeters F M, Morelle M and Moshchalkov V V 2005 Phys. Rev. B 71 184502

[33] Kato R, Enomoto Y and Maekawa S 1991 Phys. Rev. B 44 6916

[34] Kato R, Enomoto Y and Maekawa S 1993 Phys. Rev. B 47 8016

[35] Gropp W D, Kaper H G, Leaf G K, Levine D M, Palumbo M and Vinokur V M 1996 J. Comput. Phys.

123 254

[36] Silhanek A V, Gladilin V N, Van de Vondel J, Raes B, Ataklti G W, Gillijns W, Tempere J, Devreese J T and

Moshchalkov V V 2011 Supercond. Sci. Technol. 24 024007

[37] Gladilin V N, Tempere J, Devreese J T, Gillijns W and Moshchalkov V V 2009 Phys. Rev. B 80 054503

[38] Buzdin A and Daumens M 1998 Physica C 294 257

[39] de Souza Silva C C, Van de Vondel J, Zhu B Y, Morelle M and Moshchalkov V V 2006 Phys. Rev. B 73 014507

New Journal of Physics 15 (2013) 063022 (http://www.njp.org/)